Upcoming SlideShare
×

# 30320130403002

243 views

Published on

Published in: Technology, Business
0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
Your message goes here
• Be the first to comment

• Be the first to like this

Views
Total views
243
On SlideShare
0
From Embeds
0
Number of Embeds
2
Actions
Shares
0
2
0
Likes
0
Embeds 0
No embeds

No notes for slide

### 30320130403002

1. 1. International Journal of Design and Manufacturing Technology (IJDMT), ISSN 0976 – 6995(Print), INTERNATIONAL JOURNAL OF DESIGN AND MANUFACTURING ISSN 0976 – 7002(Online) Volume 4, Issue 3, September - December (2013), © IAEME TECHNOLOGY (IJDMT) ISSN 0976 – 6995 (Print) ISSN 0976 – 7002 (Online) Volume 4, Issue 3, September - December (2013), pp. 08-14 © IAEME: http://www.iaeme.com/IJDMT.asp Journal Impact Factor (2013): 4.2823 (Calculated by GISI) www.jifactor.com IJDMT ©IAEME PREDICTION OF LIMITING DRAW RATIO (LDR) BY USING FINITE ELEMENT METHOD (FEM) BASED SOFTWARE SIMULATIONS Namraj Garhewal1, Pravin Kumar Singh2 1 M. Tech Scholar, Department of mechanical engineering, University institute of technology, Barkatullah University, Bhopal, India. 2 Assistant professor, Department of mechanical engineering, University institute of technology, Barkatullah University, Bhopal, India. ABSTRACT Deep drawing process of sheet metal is mostly used for cup shape forming. For cup shape forming a limiting value of blank diameter, for which value we can successfully draw a cup. If the punch diameter, efficiency factor and all the process parameters are fixed, and we increase that value of blank diameter, then the limit value of failure can be obtained. The ratio of maximum blank diameter which is successfully drawn to the punch diameter is called LDR (Limiting Drawing Ratio). Analytically we can find out the value of LDR. We can find out the value of LDR also from Experiments. But there is a big difference between the analytical value and experimental value. The value of LDR is also find out by the software simulation of deep drawing process and this value is very close to the experimental value of LDR. So with the help of simulation we can predict the value of LDR, which can reduce the experimental set up cost. We are using RADIOSS software for FEM simulation of deep drawing process. The work presented in this paper focuses on the concept of deep drawing. All the materials considered are elastic. The material used is SAE_J2340_CR_210A_Dent_Resist. The software used for the simulation and analysis is RADIOSS software. For the analysis, constant process parameters like punch speed; blank holding force, punch travel and friction co-efficient have been considered. On these parameters different blank diameters, within 0.5 mm interval, have been considered in order to find out various safe, marginal and failure conditions for different materials respectively. In this simulation, the displacement of material under deep drawing of cup shape, plastic strain on different sections of the cup and % age thinning have been analyzed. Safe value, marginal value and the failure limit of various materials with different diameters taking into consideration have been observed. It has also been observed that the zone of minimum 8
2. 2. International Journal of Design and Manufacturing Technology (IJDMT), ISSN 0976 – 6995(Print), ISSN 0976 – 7002(Online) Volume 4, Issue 3, September - December (2013), © IAEME displacement (dark blue color of the displacement diagram) varies from higher to lower progressively safe condition towards failure condition. And this dark blue zone goes on decreasing progressively. With the help of this paper, it has been shown that the value of LDR by simulation is very close to value obtained of LDR by experimental value (published data). With the value of LDR, the failure condition of different materials in deep drawing process has been predicted. Keywords: Deep drawing, FEM simulation, LDR, Forming Limit Diagram, RADIOSS. I. INTRODUCTION The ability to produce a variety of shape from sheet of metal at high rate of production is one of the outstanding qualities of the sheet metal working processes. The importance of sheet metal working process in modern technology is due to the ease with which metal may be formed into useful shapes by plastic stage deformation process in which the volume and mass of metal are conserved and metal is only displaced from one position to another. Deep drawing is one of the widely used sheet metal working process to produce cup shaped component at very high rate. Sheet metal forming process serves as a basic test for the sheet metal formability. In deep drawing process a sheet of metal is used to form cylindrical component by pressing the central portion of the sheet into die opening to form the metal into desired shape. The efficiency of deep drawing process depends upon many parameters and the choice of these parameters is very important to achieve the high drawability. The deformation of sheet metal in deep drawing can be quantitatively estimated by dwaw ratio (DR), which is defined as the ratio of initial blank diameter to the diameter of the cup drawn from the blank (approximately equal to punch diameter). For a given material there is a limiting draw ratio (LDR), representing the largest blank that can be drawn through the die successfully. The drawability of the metal depends on two factors. 1. The ability of material in the flange region to flow easily in the plane of sheet under shear. 2. The ability of side wall material to resist deformation in the thickness direction. The mechanical properties which are considered to the important in sheet formability are average plastic strain ratio (‫ )ݎ‬and the strain hardening component (n). The strength of final part as measured by yield strength must also be considered. Take both the above mentioned factors into account it is desirable in the drawing operation to minimize material flow in the plane of the sheet and to maximize resistant to material flow in direction perpendicular to the plane of the sheet. The flow strength of sheet metal in the thickness direction is difficult to measure, but the plastic-strain ratio r compares strengths in the plane and thickness directions by determining true strains in these directions in a tension test. For a given metal strained in a particular direction, r is a constant expressed as: r= ߳௪ ߳௧ Where ߳௪ = True strain in width direction. ߳௧ = True strain in thickness direction. 9